1

**Influence of Constituents on Creep **

**Properties of SiC/SiC Composites**

**R. Bhatt**

**Ohio Aerospace Institute, Cleveland, OH, 44135**

**Ohio Aerospace Institute, Cleveland, OH, 44135**

**J. DiCarlo**

**Distinguished Research Associate**

**Distinguished Research Associate**

**NASA Glenn Research Center**

**NASA Glenn Research Center**

**.**

**.**

**Research Supported by the**

**Research Supported by the**

**NASA **

**Transformational Tools & Technologies (TTT) Project**

**Presentation at HTCMC-9,**

**Toronto, Canada, June 26 – July 1, 2016**

**OBJECTIVE:**

• **With the overall goal of developing higher temperature SiC/SiC CMC for **
**improved aero-propulsion engines, the objective of this study was to **

**understand the creep-limited upper use temperatures of SiC/SiC CMC with **
**currently available fiber and matrix constituents by measuring and **

**modeling the high-temperature creep behavior of CMC containing two **
**high-performance SiC fibers and various SiC-based matrices.**

**SiC/SiC CMC CONSTITUENT FOCUS:**

• **SiC Fibers:**

• **Hi-Nicalon-S (HNS) (current best creep-resistant fiber) **

• **SylramicTM _{-iBN (}_{iBN}_{) (slightly less creep-resistance, but higher }**

**thermal conductivity and capable of higher temperatures w/o strength **
**loss for matrix improvement by CMC heat treatment)**

• **SiC-based Matrices:**

• **Full Reaction-Formed SiC by polymer decomposition + Si Melt **
**Infiltration (Full RFMI)**

• **Full CVI SiC (Full CVI) **

• **Partial CVI SiC with partial SiC slurry and Non-Reactive Si Melt **
**Infiltration (Partial CVI-NRMI)**

• **Full Polymer-derived SiC with CVI Si _{3}N_{4}/BN fiber coatings (Full PIP)**

2

**Presentation Overview**

**Presentation Overview**

**EXPERIMENTAL:**

• **Focus on 2D-balanced SiC/SiC CMC with both straight and 5HS woven **
**fibers**

• **Measure on-axis creep behavior of CMC at constant stresses and constant **
**temperatures of 1315, 1400, and 14500 _{C in lab air. CMC stresses were kept }**

**below 110 MPa (16 ksi) to assure in most cases no matrix cracking on **
**initial loading.**

**MODELING:**

**Use CMC creep data and previously determined empirical models for the **
**creep behavior of the HNS, iBN, and the CVD-derived Ultra SCS fibers to:**

• **Understand the creep-controlling constituent for each CMC type.**

• **Develop an empirical understanding and analytical equations where **
**possible for the creep behavior of the various matrix types.**

• **Develop methodology for predicting the creep-limited upper use **
**temperatures (T*) for each CMC type under constant stress and **
**temperature conditions.**

**Approach**

**Approach**

**Background on NASA Fiber **

**Background on NASA Fiber**

**Creep Studies**

**Creep Studies**

**Relevant to the**

**Relevant to the**

**Creep Behavior for the Various **

**Creep Behavior for the Various**

**SiC/SiC CMC Types**

**SiC/SiC CMC Types**

5

**Typical Tensile Creep Behavior**

**Typical Tensile Creep Behavior**

**of Near-Stoichiometric Polymer-derived SiC Fibers**

**of Near-Stoichiometric Polymer-derived SiC Fibers**

• **Near stoichiometric polymer-derived SiC fibers with ~ equiaxed **
**grains, like HNS and iBN, show elastic behavior followed by a small **
**primary (transient) stage and a secondary (steady-state) creep stage. **
• **The primary stage increases linearly with stress, whereas the **

**typically larger steady-state stage increases to the third power with **
**stress, but decreases linearly with increasing grain size. **

6

**Ultra Fiber Creep in air at 14000 _{C and 278 MPa (40 ksi)}**

**True**
**Creep **
**Strain**
**Time, hours**
**As-Produced **
**After 1-hr 1800o _{C Anneal}**

**Typical Tensile Creep Behavior of the **

**Typical Tensile Creep Behavior of the**

**Near-Stoichiometric CVD-derived Ultra SCS Monofilament **

**Near-Stoichiometric CVD-derived Ultra SCS Monofilament**

**SiC Fiber**

**SiC Fiber**

• **Unlike the polymer-derived SiC fibers with ~ equiaxed grains, the CVD-derived **
**Ultra fiber only displays a primary (transient) stage with t1/3 _{and linear stress }**

**dependences. This is probably related to the elongated transverse grains in these **
**fibers, which grow in size with annealing above 14000 _{C along with free Si removal, }**

**thereby increasing fiber creep resistance.**

• **Because of microstructural similarities, it is assumed that the **
**stress-time-temperature creep behavior of the CVD-derived Ultra fiber should be useful in **
**understanding the creep behavior of a CVI SiC matrix constituent.**

7

**Polymer-derived: ε _{s }(%) =**

**A · θ / d**

**(T) where**

**θ =**

**3**

_{· t · exp (-}

_{B}

_{/T), }**CVD-derived: ε _{p}**

**(%) = C (T) · θ1/3**

**d** **= grain size (nm), ** **= stress (MPa), t = hours, T = Kelvin**

**Best-Fit Creep Parameters for Straight SiC Fiber Types**

**Best-Fit Creep Parameters for Straight SiC Fiber Types**

**under constant Stress and Temperature**

**under constant Stress and Temperature**

**d**
**(nm)**
**A**
**(%.K. nm/MPa3 _{.hr)}**

**B**

**(K)**

**C**

**(%/ MPa. hr1/3 )**

**HNS**

**20**

**2.2 x 1016**

_{97900}**iBN**

**~ 200**

**4.5 x 1017**

_{97900}**Advanced SiC Fiber** **400** **2.2 x 1016** _{97900}

**Ultra (as-produced)** _{97900}**9 x 104**

**Ultra (16000 _{C anneal)}**

**97900** **2 x 10 4**

**Ultra (18000 _{C anneal)}**

**97900** **9 x 10 3**

• **The theoretical Advanced polymer-derived SiC fiber is projected to mimic **
**the Hi-Nicalon-S fiber, but with reduced oxygen content and ~400 nm **
**grains distributed uniformly in the fiber to increase creep resistance.**

• **The B** **parameter for all fiber types corresponds to a steady-state creep **
**activation energy of Q = 8.31** **B = 814 kilo-joules (diffusion of C in SiC).**

• **For 2D-woven architectures with stress-riser bends in small-diameter **
**fibers, the A constants increase by ~ 2 to 3 depending on fiber diameter **
**and weaving angle.**

**Creep Data for the Various **

**Creep Data for the Various**

**SiC/SiC CMC Types**

**SiC/SiC CMC Types**

**CMC stress = 69 MPa**
_{f}= 630 MPa**CMC stress = **** _{c}= 103 MPa**

_{f}= 940 MPa**(**

***)3**

_{rate }**increase**

**Creep Behavior at 1400**

**Creep Behavior at 1400**

**0**_{C for CMC with Full RFMI matrix }

_{C for CMC with Full RFMI matrix }**and 2D-balanced non-woven HNS architecture (f**

**and 2D-balanced non-woven HNS architecture (f**

_{o}**= 0.11) **

**= 0.11)**

9

• **CMC creep strain before rupture is linear with time and increases with **
**CMC stress to the third power indicating that although this material is **
**not cracked, its creep is controlled entirely by the Hi-Nicalon-S fiber **
**even though it has a low on-axis fraction of ~11%. **

• **Thus the RFMI matrix is very creep prone at 14000 _{C and the }**

**creep-limited upper use temperature for this CMC type is controlled entirely by **
**the fiber creep behavior under a stress based on the total CMC stress. **

**Total Strain,**
**%**

### •

**Using steady-state creep equations and associated parameters for **

**the creep-controlling polymer-derived SiC fiber, one can then **

**calculate the CMC T* with this fiber by:**

**T***

**(kelvin) = **

**B**

**/ln{( **

**A/d**

**)·**

###

_{f }3**·t/ε*} **

**Where **

###

_{f}**= (**

###

_{c}**/ f**

_{o}**) = fiber initial stress, t = desired CMC component **

**service life, and ε**

*****

_{= max strain (%) that CMC component can tolerate. }

_{= max strain (%) that CMC component can tolerate. }

### •

**As an example, assume **

###

_{f}**= 400 MPa (**

###

_{c}**= 100 MPa, f**

_{o}**= 0.25), t = **

**1000 hr, and ε**

*****

_{= 0.2%, a value often quoted for metal turbine }

_{= 0.2%, a value often quoted for metal turbine }

**components. Then ~**

**T***

**for straight polymer-derived SiC fibers are:**

### •

**These T* values for RFMI matrices should also hold for a fully **

**cracked CMC at t = 0, but such a case may be undesirable due to **

**fiber environmental attack. Also beneficially, these T* do not take **

**the CMC above 1414**

**0**

_{C where melting and diffusion of the free }

_{C where melting and diffusion of the free }

**silicon in the matrix can cause internal CMC damage.**

10

**Calculating Creep-Limited UUT (T*) for SiC/SiC CMC **

**Calculating Creep-Limited UUT (T*) for SiC/SiC CMC**

**containing highly Creep-Prone Matrices like Full RFMI**

**containing highly Creep-Prone Matrices like Full RFMI**

**Hi-Nicalon-S** **Sylramic-iBN** **Advanced**
**T*** **13300 _{C}**

_{1310}0_{C}

_{1410}0_{C}**Creep Behavior at 1315 and 1450**

**Creep Behavior at 1315 and 1450**

**0**_{C for CMC with}

_{C for CMC with}**Full CVI matrix (~50%) and 2D-balanced 5HS-woven HNS **

**Full CVI matrix (~50%) and 2D-balanced 5HS-woven HNS**

**fiber architecture (f**

**fiber architecture (f**

_{o}**= 0.17)**

**= 0.17)**

11

• **CMC creep strain follows t1/3** _{time dependence, indicating that its creep is }

**primarily controlled by the Full CVI SiC matrix.**

• **Assuming a CVI SiC content of 50%, the transient creep equation for the **
**Ultra fiber, ε _{p}(%) = (C)[**

_{m}] [ t x exp (-B/T)]1/3_{,}**and **_{m }equal to the full CMC stress on the matrix, above CMC curves yields

**C** **parameters at 1315 and 1450****0**_{C that match those measured for the Ultra }**fiber at these temperatures, indicating that the Ultra fiber creep equation **
**and parameters can be used to predict SiC/SiC CMC on-axis creep with Full **
**CVI matrices and current polymer-derived SiC fibers.**

**(Time, hrs)1/3**
**Cr**
**eep **
**Str**
**ai**
**n**
**, %**
**0**
**0.05**
**0.1**
**0.15**
**0.2**
**0.25**
**0.3**
**0** **2** **4** **6** **8**
**1315C, 69 MPa **
**ε _{p}= 0.0135 t1/3**

**1450C, 86 MPa**

**ε**

_{p}= 0.0391 t1/3**Time, hrs**

**1450C, 86 MPa**

**1315C, 69 MPa**

**To**

**tal**

**T**

**ensile**

**Str**

**ai**

**n**

**, %**

**CMC Creep Behavior at 1315 and 1400**

**CMC Creep Behavior at 1315 and 1400**

**0**_{C for CMC with}

_{C for CMC with}**Partial CVI-NRMI matrix and 2D-balanced 5HS-woven **

**Partial CVI-NRMI matrix and 2D-balanced 5HS-woven**

**iBN architectures (f**

**iBN architectures (f**

_{o}**= 0.21) **

**= 0.21)**

12

• **CMC Creep data with Partial CVI-NRMI also follows a t1/3** _{dependence }

**indicating initial control by CVI SiC matrix with content of only ~22%.**

• **For longer times the data starts to bend upward, suggesting either matrix **
**cracking or MI silicon diffusing into CVI SiC making it more creep prone.**

• **At 13150 _{C, CMC with Partial CVI-NRMI matrix is initially more creep resistant }**

**(reduced C parameter) than the CMC with as-produced Full CVI matrix, which **
**can be explained by the Partial CVI matrix being annealed during the NRMI **
**process near 14000 _{C. }**

**(Time, hrs)1/3**

**Cr**

**eep**

**Str**

**ai**

**n**

**, %**

**13150**

_{C, 103 MPa }**ε**

_{p}= 0.0121 t1/3**14000**

_{C, 103 MPa }**ε**

_{p}= 0.0329 t1/3**To**

**tal**

**T**

**ensile**

**Str**

**ai**

**n**

**, %**

**Time, hrs**

**13150**

_{C, 103 MPa }**14000**

_{C, 103 MPa }**Creep Behavior at 1454**

**Creep Behavior at 1454**

**0**_{C for CMC with}

_{C for CMC with}**Full PIP matrix and 2D-balanced 5HS-woven iBN **

**Full PIP matrix and 2D-balanced 5HS-woven iBN**

**architecture (f**

**architecture (f**

_{o}**= 0.25%) **

**= 0.25%)**

13

• **Like CMC with CVI SiC, creep data for CMC with Full PIP matrix produced at **
**~16000 _{C also follows a t}1/3**

_{dependence at low stress for long time at 1454}0_{C. }• **Mechanism for similar behavior with CVI matrices is uncertain since porous **
**PIP matrix is expected to carry little load and behave like the creep-prone **
**fine-grained polymer-derived SiC fibers.**

• **One possible mechanism is that the iBN fibers are coated with a dual layer of **
**CVI Si _{3}N_{4}**

**over BN (Mod-1 coating) with the CVI Si**

_{3}N_{4}**coating having**

**significant volume fraction and potentially high creep resistance like CVI SiC.**

**1454C, 69 MPa **
**ε _{p}= 0.0408 t1/3**

**1454C, 69 MPa**

**Cr**

**eep**

**Str**

**ai**

**n**

**, %**

**(Time, hrs)1/3**

**To**

**tal**

**T**

**ensile**

**Str**

**ai**

**n**

**, %**

**Time, hrs**

**Temperature Dependence for “**

**Temperature Dependence for “**

**C**

**C**

**” parameter in the Primary **

**” parameter in the Primary**

**Creep Equation for CVI-derived Fibers and Matrices**

**Creep Equation for CVI-derived Fibers and Matrices**

**Assuming the creep of uncracked SiC/SiC CMC with CVI-derived matrices is **
**controlled entirely by the matrix, the CMC creep behavior can be closely **
**predicted from primary creep strain equation for the CVI-derived Ultra fiber,**

**ε (%) = C(T)[ **_{m}**t 1/3** _{exp (-}_{B}_{/3T)}

**its “C” dependence on max anneal or creep temperature, and a stress on **

### •

**Using the primary stage creep equations and associated **

**parameters for the CVD-derived Ultra SCS fiber, one can then **

**calculate **

**T***

**for the SiC/SiC CMC with a CVI matrix content V**

_{m}**by:**

**T***

**(kelvin) = **

**B**

**/3 ln (**

**C**

###

_{m}**t **

**1/3**

**/ε**

*****

_{)}

_{)}

**Here **

###

_{m}**= (**

###

_{c}**/ V**

_{m}**) = matrix stress, t = desired CMC component **

**service life, and ε**

*****

_{= max creep strain (%) that CMC component can }

_{= max creep strain (%) that CMC component can }

**tolerate. **

### •

**Assuming **

###

_{c}**= 50 MPa to avoid initial matrix cracking, V**

_{m}**= 0.20 **

**(Partial) to 0.50 (Full), t = 1000 hr, and ε**

*****

_{= 0.2%, }

_{= 0.2%, }

_{T*}

_{T*}

_{for as-produced }

_{for as-produced }

**and 1800**

**0**

_{C-annealed CVI SiC matrices are estimated as follows:}

_{C-annealed CVI SiC matrices are estimated as follows:}

### •

**Note that if the CMC with CVI matrix should crack at the high T*, the **

**crack-bridging creep-prone polymer-derived fibers within a short **

**time will probably cause undesirable CMC deformation and/or **

**rupture. **

.15

**Calculating Creep-Limited UUT (T*) for SiC/SiC CMC **

**Calculating Creep-Limited UUT (T*) for SiC/SiC CMC**

**containing Full or Partial CVI Matrices**

**containing Full or Partial CVI Matrices**

**As-produced**
**V _{m}**

**= 0.20**

**As-produced**

**V**

_{m}**= 0.50**

**18000**

_{C Annealed}**V**

_{m}**= 0.20**

**18000**

_{C Annealed}**V**

_{m}**= 0.50**

**T***

**12900**

_{C}

_{1365}0_{C}

_{1490}0_{C}

_{1580}0_{C}**Summary and Conclusions**

**Summary and Conclusions**

• **For the current SiC/SiC CMC types addressed in this study, it was determined **
**that at high temperatures no close creep match between the fiber and matrix **
**existed in order that both could carry the on-axis CMC load for long times. **
**For example, for CMC with Full RFMI matrices, the HNS and iBN fibers **

**controlled CMC creep; and for CMC with Full CVI, Partial CVI-NRMI, and Full **
**PIP matrices, the matrix controlled CMC creep.**

• **At high temperatures, it was shown that obtaining a fiber-matrix creep match **
**with the best creep-resistant polymer-derived SiC fibers may not be possible **
**since they display creep strain that follows time to the first power; while the **
**CVI-derived SiC matrices follow time to the 1/3 power.**

• **Using previously determined fiber creep equations, it was also shown that for **
**a CMC 1000 hour service life and a 0.2 % creep strain limit, the creep-limited **
**upper use temperature T*** **for Full RFMI composites was ~13000 _{C for the HNS }**

**and iBN fibers and at best 14000 _{C if an Advanced polymer-derived SiC fiber }**

**could be developed.**

• **Likewise, using a previously determined creep equation for the **

**large-diameter CVI-derived Ultra fiber, it was shown that for un-cracked CMC with **
**CVI-derived matrices under the same service requirements, the T*** **could be **
**as high as 16000 _{C dependent on the CMC creep or pre-anneal temperature.}**

• **All these results support the need for development of small-diameter **
**CVI-derived SiC fibers to match the creep behavior of CVI-CVI-derived matrices, and **
**thus obtain SiC/SiC CMC with highest creep resistance and T***.